Paste 2017, Beijing, China 190
Translating paste backfill admixture results from the
laboratory into the field
Fabian Erismann Sika Services, Switzerland
Christophe Kurz Sika Technology, Switzerland
Martin Hansson Sika Sweden, Sweden
John Almas Sika China, China
Paste backfill admixtures have been used in mine paste backfill plants for many years. Their use has been
targeted to improve specific properties of the paste such as the water and binder requirements for a certain
workability and strength, to improve the slump and flow characteristics, to reduce paste line pressures or to
enhance the stability of the paste in order to reduce risk of line blockages.
The economic justification for the use of paste backfill admixtures was in earlier days questioned in projects
across the world as visible operational cost improvements could not always be clearly demonstrated. With
the development of new generation paste backfill admixtures over the past years, the economic benefits can
now be clearly demonstrated. State of the art admixtures can impact the economics of paste plants and
associated infrastructures significantly. Sika together with its partners utilised lessons learned from concrete
admixtures and translated this knowledge in order to apply the same p
rinciples in paste plants across the globe. Significant cement reduction targets of up to 50% could be reached,
which changed the perception towards the use of admixtures significantly. Translating initial laboratory
results into the field remains one of the key challenges. This paper will outline this critical transition from
laboratory into the field using three case studies from mines located in Europe and Africa. The results obtained
in the laboratory can often be translated into the real world with minor variances of the critical parameters
such as the admixture dosage, slump and strength development but we also show that there are exceptions.
Understanding the actual origin and composition of the paste remains critical for the selection of the best
performing paste backfill admixture and for a successful transition from promising laboratory results into the
Utilizing dewatered tailings for underground backfilling is becoming the standard in many underground cut
and fill and long hole stoping operations globally. At the same time, increased cement consumption and rising
operating costs represent a major issue in many mines. Optimizing the cost performance of the backfilled
mix as well as the reliability of the backfill plant has become a major objective in recent years. The
introduction of admixtures into the paste backfill mix has been successful in several mining operations. The
selection of the right admixture and the implementation of the admixture into the daily operation are critical
to fully utilize the potential of admixtures and to materialize the targeted cost savings. The first step for
evaluating admixtures for a given paste plant is successful laboratory trial with the tailings and binder in use.
191 Paste 2017, Beijing, China
Once laboratory trials have been successfully completed, the system needs to be proven reliable in large
scale, via on site field trials at the paste plant. This transition from the laboratory into the field is critical.
Based on three case studies we will outline this transition methodology. The three case studies cover
completely different ore deposits from where the wetted-out tails were sourced, mixed with binder and
admixture and backfilled into underground stopes. Remaining within the workability limits as well as reaching
the required strength values after a given time are the defining parameters that had to be fulfilled and within
this range, the mix design was cost-optimized.
2 Admixture selection process
Selecting effective admixtures for each paste was the first and most important step in the cost optimization
process. The precondition for a successful selection process is a good and detailed understanding of the
tailings and the binder composition. The geochemical characteristic of the tailings, by far the largest
component of the paste mix by volume, has a dominating effect on the effectiveness of a chosen admixture
(Erismann et al., 2016). Understanding the geological origin of the ore deposit and hence the tailing
mineralogical composition and sieve curve is critical. Over the past years, Sika developed an extensive
database from tailings across the globe, covering most deposit types that are today mined with selective
underground methods that normally utilize cemented paste backfilling. This database is the foundation of
how we approach backfill plants and provides very useful selection criteria in order to streamline this critical
selection process. Once the right admixture has been identified and the best cost performing dosage has
been determined in the laboratory, the next step is to prove the upgraded paste mix design in the field.
3 Laboratory trials
Laboratory trials were set up in a way to be easily reproducible in the paste laboratory at the mine site with
minimal equipment needs. Standard Hobart concrete mixers as well as casted mortar bars were used to test
different mix designs including compressive strength testing. Transparent cylinders are used for bleeding
tests. Workability of the paste is tested by using half sized concrete Abrams cones. Compressive strength
testing takes place according to the mines requirement but usually after 7 and 28 days and sometimes also
after 56 days. Promising admixtures usually lead to strong increase in slump and slump-flow of the paste mix
at moderate dosages (Erismann et al., 2016). Such a slump increase of the reference mix is usually a pre-
condition to upgrade the paste mix design by reducing the water content of the paste. Once the best cost
performing admixture has been identified, the water content is reduced by such extent that the workability
limits of the paste (required slump) are maintained. Once the upgraded compressive strength results have
been obtained, the binder is reduced to such extent that the overall compressive strength requirement is
within the accepted boundaries.
4 Onsite trials
Once the optimized mix design has been identified, the new system needs to be tested on a large scale in
order to verify the cost savings under real conditions. The shear energy as well as the scale of materials mixed
is obviously much different when comparing laboratory trials to field trials. However, the approach at the
paste plant is very much the same as in the laboratory. The admixture is dosed directly into the wetted-out
mix using standard dosing equipment as seen in Figure 1. The admixture is dosed into the paste hopper or
directly into the paste mixer. In order to prevent an overdosing of the system, the starting dosage is around
50% of the actual dosage determined in the laboratory. Once this dosage has been added for a few cycles (in
batched paste plants) or for a certain time interval (for continuous paste plants) the dosage can be step-wise
Paste 2017, Beijing, China 192
increased until the targeted dosage from the laboratory trials has been reached. Standard paste cylinders are
filled with the different paste mixes and stored under controlled conditions for compressive strength testing.
Figure 1 Admixture set-up at the paste plant. Bulk containers are coupled to the dosing unit (right side of image)
that is coupled to the control system of the paste plant. The admixture is then pumped to the dosing
5 The case studies
The following three case studies have been selected to illustrate the successful transition from the laboratory
to the paste plant.
Polymetallic zinc-lead-copper SEDEX deposit in Northern Europe.
Polymetallic, epithermal gold-copper deposit in Eastern Europe.
Orogenic gold deposit in West Africa.
These three deposits have a completely different origin, deformation and alteration history and hence can be
seen as completely independent geological systems. These differences become clear when looking at the
alteration mineralogy of the deposit, the metallurgical composition as well as the grind size needed in order
to liberate the minerals of interest. All of these parameters have a defining impact on how the admixtures
will interact with the tailings derived from these three deposits. As a result of these differences, different
binders were used in varying quantities in order to obtain the required compressive strengths. These case
studies and the requirements of the paste backfill operation are described briefly below.
5.1 Polymetallic zinc-lead-copper SEDEX deposit in Northern Europe